Lamina Coordinate Transformation for Arbitrary Orientation
 Lamina Coordinate Transformationfor Arbitrary Orientation
 Formula Home Composites Intro. to Composites Lamina Properties Stress-Strain Relations Principal Direction Material Constants Coord. Transformation Arbitrary Orientation Laminated Composites FRC Calculators Est. Material Const. Lemina Stiffness Leminate ABD Material Data Elastic Moduli Resources Bibliography
 Home Membership Magazines Forum Search Member Calculators
 Materials Design Processes Units Formulas Math
 Coordinate Transformation is Necessary The generalized Hooke's law of a fiber-reinforced lamina for the principal directions is not always the most convenient form for all applications. Usually, the coordinate system used to analyze a structure is based on the shape of the structure rather than the direction of the fibers of a particular lamina. For example, to analyze a bar or a shaft, we almost always align one axis of the coordinate system with the bar's longitudinal direction. However, the directions of the primary stresses may not line up with the chosen coordinate system. For instance, the failure plane of a brittle shaft under torsion is often at a 45° angle with the shaft. To fight this failure mode, layers with fibers running at ± 45° are usually added, resulting in a structure formed by laminae with different fiber directions. In order to "bring each layer to the same table," stress and strain transformation formulae are required.
 Coordinate Transformation of Stress-Strain Relations for Lamina If we define the coordinate transformation matrix as and The coordinate transform of plane stress can be written in the following matrix form: Similarly, the strain transform becomes Please notice that the tensor shear strain is used in the above formula. Suppose we define the engineering-tensor interchange matrix [R] then The stress-strain relations for a lamina of an arbitry orientation can therefore be derived as detailed below. where the stiffness matrix is defined as The complicance matrix is therefore The individual components of the stiffness and compliance matrices can be found here.